Abstract
We investigate the thickness optimization for maximum currentinduced spinorbit torque (SOT) generated by topological surface states (TSS’s) in a bilayer system comprising of a ferromagnetic layer coupled to a thin topological insulator (TI) film. We show that by reducing the TI thickness, two competing effects on the SOT are induced: (i) the torque strength is stronger as the bulk contribution is decreased; (ii) on the other hand, the torque strength becomes suppressed due to increasing hybridization of the surface states. The latter is attributed to the opposite helicities of the coupled TSS’s. We theoretically model the interplay of these two effects and derive the optimal TI thickness to maximize the spin torque, which is estimated to be about 3–5 nm for typical Bi_{2}Se_{3} films.
Introduction
Spin torque is one of the most actively researched topics in spintronics. In spinorbit coupling (SOC) systems, the spinorbit torque (SOT) comprises of two types: fieldlike torque^{1,2,3,4,5,6} and dampinglike torque^{7, 8}. The SOT strength scales with the SOC strength, therefore one can obtain a large SOT signal in strong SOC systems, such as heavy metal/ferromagnet (Pt/Co)^{9} and topological insulators (TI)^{10,11,12}.
Topological insulators possess strong SOC which translates to a large SOT effect. Moreover, the spinlocked topological surface states of TI are robust under timereversal symmetric impurity scattering. These factors enable TI to be one of the most promising candidates for SOT devices. When a current is passed onto the TI surface (interface), a nonequilibrium spin density will be induced on that surface^{10}, which is directed inplane and perpendicular to the applied current as a result of the spinmomentum locking of the surface states^{10}, similar to the RashbaEdelstein effect^{13}. Thus spin accumulation is proportional to the charge current flowing on the TI surface^{1, 3, 10}. In addition, an outofplane spin density can be generated due to the Berry curvature of the spin texture in the momentum space^{8, 14, 15}, and due to the presence of the hexagonalwarping effect^{16}. The two components, inplane and outofplane spin density, are responsible for inducing an outofplane and inplane torques, respectively.
In the study of currentinduced SOT, spin torque efficiency (ratio of torque strength and current density in the TI  \({\mathscr{T}}/{j}_{{\rm{TI}}}\), which is equivalent to spin Hall angle j _{ s }/j _{TI}) is a crucial quantity. In 3D TI’s, the surface state has a finite thickness and usually extends into the bulk material, up to 1 nm from the TIvacuum interface^{11, 17}, and the current is supposed to flow entirely in the surface channel in ideal TI. However, in practical 3D TI’s, the bulk is not totally insulating^{18}, and thus the current in the TI can flow both in the surface and bulk channels. Since the bulk states do not exhibit any spinmomentum locking, TI with a large bulk conductance will induce a smaller torque on an adjacent ferromagnetic (FM) layer. Therefore, it is obvious that one has to reduce the TI thickness to reduce the relative contribution of the bulk^{19,20,21}, and enhance the torque efficiency. But how far can the thickness of a TI film be reduced?
Normally, a 3D TI film comprises of two surfaces (top and bottom surfaces, for example). In a typically thick TI film, the two surfaces are uncorrelated, i.e., the transport on one surface will not affect the other. However, if the film is made very thin, i.e., its thickness is comparable to the decay length of surface states, the two surface states become hybridized^{17, 22,23,24}. This hybridization is quantified by a tunneling coupling constant (Δ), which is thus a function of the TI thickness. Generally, Δ is larger as the thickness is reduced^{17, 22, 23}. The effect of the surfaces hybridization on spin torque is as follows. When a charge current is passed onto the top surface in the xdirection, it can leak to the bottom surface through the tunneling effect^{25}. While the current on the top surface induces a spin accumulation in the ydirection, its bottom counterpart induces a spin accumulation in the opposite, i.e., –ydirection, since the two surface states have opposite helicities. As a result, the total spin accumulation is reduced with the hybridization effect. Thus, the spin torque is also reduced as the TI thickness is reduced. This dependence will be formulated subsequently in this paper.
From the above, we may surmise that the reduction in the TI thickness has two competing effects on the spin torque: (i) the torque strength is stronger as the bulk contribution is decreased; (ii) on the other hand, the torque strength becomes suppressed due to increasing hybridization of the surface states. Therefore, there is an optimal value of TI thickness which would maximize the torque efficiency. Thus, the aim of this study is to investigate the spin torque in TI film in the presence of the hybridization effect. We will formulate the relation between spin torque and TI thickness, from which we derive the optimal value of the thickness to maximize the torque.
Results
Spin torque in thick TI films
We will first formulate the spintorque induced by charge current in a coupled FM/TI bilayer system in the absence of intersurface hybridization. In a thick TI film, only the topological surface state coupled to the magnetic layer is active (the top TSS in Fig. 1), whereas the other has no effect and thus can be ignored (the bottom TSS). The system is described the by following Hamiltonian:
where the first term is the Dirac Hamiltonian of the active topological surface state \({ {\mathcal H} }_{{\rm{TI}}}=\hslash {v}_{{\rm{F}}}({\bf{k}}\times \hat{z})\cdot \hat{\sigma }\) with v _{F} being the Fermi velocity, \(\hat{\sigma }\) is the vector of the Pauli matrices. The last term is the sd exchange interaction between itinerant electrons and magnetization with J _{ex} being the exchange constant, and m is unit vector of the magnetization which is assumed to be inplane. We can rewrite Eq. (1) to express electron spin in an effective magnetic field as \( {\mathcal H} ={\bf{b}}\cdot \hat{\sigma }\), where \({\bf{b}}=\hslash {v}_{{\rm{F}}}({\bf{k}}\times \hat{z})+{J}_{{\rm{ex}}}{\bf{m}}\). The eigenenergies are found as
where s = ±1 which is for majority and minority electron, respectively, and we have used the fact that m = 1. For a given value of momentum k, Eq. (2) can be considered as the energy of the magnetic system. Thus, the torque field acting on the magnetization can be found by taking the functional derivative of \({ {\mathcal E} }_{s}({\bf{k}})\), i.e.^{1,2},
In the above, n is the charge density, and M _{ s } is the saturated magnetization. Let us first consider the contribution from the lower band. In this case, from Eqs (2) and (3), the torque field is
The upper band will gives rise to an opposite torque field. To obtain the above, we have assumed the strong exchange limit, i.e., \({J}_{{\rm{ex}}}\gg \hslash {v}_{{\rm{F}}}{k}_{{\rm{F}}}\), \(b\approx {J}_{{\rm{ex}}}\), and the effective field is taken to the first order in ħv _{F} k/J _{ex}. The net torque field is found by summing over all momentum space. In the absence of applied current, the expectation value of k would vanish and so would the effective field. However, in the presence of some charge current \({{\bf{j}}}_{e}^{ss}\) that flows on the surface, the average k is finite and can be found as following. The charge current is expressed as \({{\bf{j}}}_{e}^{ss}=ne\langle {\bf{v}}\rangle \), where n is the sheet carrier density, and \({\bf{v}}=\frac{\partial H}{\hslash \partial k}={v}_{{\rm{F}}}(\hat{z}\times \hat{\sigma })\) is the velocity. In the adiabatic limit, the electron spin is mostly aligned along the effective field as \(\langle \hat{\sigma }\rangle ={\bf{b}}/b\), from which the charge current is \({{\bf{j}}}_{e}^{ss}=ne\frac{\hslash {v}_{F}^{2}}{{J}_{{\rm{ex}}}}\langle {\bf{k}}\rangle +ne{v}_{{\rm{F}}}(\hat{z}\times {\bf{m}})\). Rearranging the equation, we have
Substituting Eq. (5) into Eq. (4), we obtain the currentinduced torque field,
where \({\eta }_{0}=\frac{{J}_{{\rm{ex}}}}{e{v}_{{\rm{F}}}{\mu }_{0}{M}_{s}}\), and we have ignored the component that is parallel to m, as this does not induce torque on the magnetization itself. The field in Eq. (6) is inplane and it induces an outofplane torque on the magnetization as \({\mathscr{T}}={\bf{m}}\times {{\bf{H}}}^{{\rm{eff}}}\). Explicitly,
In practice, an applied current \({j}_{e}^{0}\) in the system is composed of three different channels: (i) surface current \({j}_{e}^{ss}\), (ii) bulk current \({j}_{e}^{b}\), and (iii) shunting current through the FM layer \({j}_{e}^{{\rm{FM}}}\), see Fig. 1(c). Therefore, from the total applied charge current \({j}_{e}^{0}\), only \({j}_{e}^{ss}\) would generate a torque field and spin torque, following Eqs (6) and (7). To obtain the relation between the surface current and the net current, we assume that the FM and TI layers have thicknesses t and d, and conductances G _{FM} and G _{TI}, respectively. The surface current is then given by
In the above, j _{ TI } is the current flowing in the TI film, \({G}_{{\rm{TI}}}^{ss}\) is the conductance of TI surface, which is assumed to be unchanged as the thickness of the TI layer d is changed. Meanwhile, the total conductance of the TI layer G _{TI} increases with d ^{18}, reflecting the increased contribution of the bulk channel. Therefore, the spin torque and torque field would generally be enhanced as d is reduced. In practice, TI films can be made very thin, i.e., down to 2 nm^{18}, and therefore one may induce large spin torque in such systems. However, as the TI film thickness is reduced to below some critical value, the property of the surface state will be changed, i.e., an energy gap is opened and the Dirac cone would disappear, as a result of the surface hybridization^{17, 21, 22, 24}. As a consequence, all spin transport effects arising from the topological surface states will be modified accordingly. The effect of surface hybridization will be considered in the following section.
Spin torque with hybridization effect
Effect of surface hybridization
In this section, we will formulate the spinorbit torque in a thin TI film with hybridization effect. In this case, both surface states (of top and bottom surfaces) are taken into account. We assume that the magnetic layer is only in contact with the top TI surface with the exchange coupling J _{ex}. The itinerant electron on the bottom surface may also couple to the FM, but with a weaker exchange coupling, which is then ignored for simplicity. In addition, we also disregard the asymmetry between the two interfaces, i.e., FM/TI and TI/substrate interfaces.
The Hamiltonian of the system is then given by^{24}
In the above, Δ represents the tunneling element (hybridization) between top and bottom surfaces, I _{2} is the (2 × 2) unit matrix. The value of Δ has an inverse relation with the thickness of the TI film, e.g., Δ = 0.05 eV for d = 5 nm film, but increases to 0.25 eV for d = 2 nm^{20}. In the range of small thickness, the tunneling element can be approximated as^{17, 22}
where B _{1} is a materialdependent parameter^{21}. Note that the Fermi velocity is also thicknessdependent. However, the variation can be neglected as its values in the thick and thin film limits only differ by the order of 0.01^{22}.
From the Hamiltonian in Eq. 9, the eigenenergies are given by
with s, τ = ±1, and
Schematic energy bands are depicted in Fig. 1(b), where the Dirac point is open in strong hybridization regime 2Δ > J _{ ex }, and it is closed otherwise. In the above, we have (2 × 2) energy bands represented by two indexes, i.e., s which has the same meaning as the spin index in the previous section, and τ which can be considered as the pseudospin index, which refers to the mixing of the top and bottom surface states. By using the same framework as in previous section, we can derive the torque field for each of the energy band as:
for the strong exchange limit (\({J}_{{\rm{ex}}}\gg \hslash {v}_{{\rm{F}}}{k}_{{\rm{F}}}\)).
If the Fermi energy E _{ F } = 0, only the two lower bands contribute to the torque field in Eq. (12), i.e., s = −1 and τ = ±1. Interestingly, the torque field in Eq. (12) does not depend on the band index τ. Therefore, the total torque field is given by \({{\bf{H}}}^{{\rm{eff}}}={\sum }_{s,\tau }{{\bf{H}}}_{s\tau }^{{\rm{eff}}}{f}_{s\tau }\), with f _{ sτ } being the distribution function for each energy band. The total torque field is given as
where
We see that the direction of the torque field in this case is still the same as in Eq. (6), i.e., in the transverse direction with respect to the applied current. However, the amplitude is now modified by a factor which is a function of the tunneling element Δ as in Eq. 14. Figure 2(a,b) depict the dependence of the torque efficiency \({\mathscr{T}}/{j}_{e}^{ss}\) on the tunneling element and the TI thickness, respectively. As expected, for a given surface state current j ^{ss}, the torque efficiency is reduced when the Δ increases, a trend which can also be discerned from Eq. (12).
Thickness optimization
As discussed in previous sections, decreasing TI thickness gives rise to two opposite effects on the spin torque: torque reduction due to the strong surface hybridization, and torque enhancement due to the weak bulk channel. In this section, we will thus derive the optimal thickness to achieve maximized spin torque.
As the thickness of TI film is reduced, the conductance of the TI film is also diminished^{18}. In extremely thin TI films, where the thickness is below 10 nm, the conductance is function of the thickness \({G}_{{\rm{TI}}}(d)={a}_{G}+{b}_{G}d\) [in units of e ^{2}/h]. Meanwhile, in the thickfilm limit, the conductance approaches an almost constant value^{18}. Experimentally, \({b}_{G}\approx 19\,{{\rm{nm}}}^{1}\) for Bi_{2}Se_{3} thin films^{18}.
The spin torque efficiency, which is the ratio between spin torque and charge current flowing in the TI, i.e., \(\theta ={\mathscr{T}}/{j}_{{\rm{TI}}}\), is then
The above expression is the product of two functions f _{1}(d) · f _{2}(d), where f _{1} (f _{2}) increases (decreases) with d. In the limit of large d, \({f}_{1}(d)\sim {\eta }_{0}\), and f _{2}(d) is relatively constant with the change in d as the conductance of the TI film is almost unchanged^{18}, which means that the torque efficiency at large TI thickness would be almost constant. However, in the range of small d, the torque efficiency is more strongly dependent on d. In Fig. 2(c), the torque efficiency first increases as the thickness is reduced. This is due to the reduction of the bulk contribution to the TI conductance, which enhances the spinpolarized current from the surface state channel. As the thickness is further reduced, the torque efficiency becomes diminished as the hybridization effect becomes the dominant factor. Thus, the torque efficiency reaches a maximum peak at some optimal value of thickness d _{max}.
Now we focus on the maximum efficiency and the corresponding thickness. Basically, these two quantities depend on system’s parameters such as B _{1}, J _{ex}. For simplicity, we consider the case where \({G}_{{\rm{TI}}}(d)={b}_{G}d\), for which the maximum efficiency can be analytically found as
corresponding to the optimal thickness of
Taking value of the tunneling parameter B _{1} = 0.1eV nm^{2}, and the exchange coupling J _{ex} = 0.1–0.5eV, the optimal thickness is estimated to be d _{max} = 2–5nm. In previous experiments^{10,11,12}, the TI films have thickness in the range of 6–20nm, which is far above the predicted optimal values. We note here that, for the maximum torque to be observed, the optimal thickness should not be below the effective thickness of the TI surface states, i.e., d _{max} > 2nm^{17, 18} (see Fig. 2(d)).
Discussion
One can check the underlying physics of the torque field reduction with the increasing surface hybridization in Eqs (13) and (14) by assuming the two surface states have the same helicity. By replacing \({ {\mathcal H} }_{{\rm{TI}}}\) by \({ {\mathcal H} }_{{\rm{TI}}}\) in the bottom right block of Eq. (9), one can find the torque field is \({{\bf{H}}}^{{\rm{eff}}}={\eta }_{0}(\hat{z}\times {\bf{k}})\), which is independent of the tunneling coupling Δ. Therefore, we can conclude that it is the coupling between surface states with opposite helicities which reduces the net torque.
As mentioned earlier, we have assumed that the FM layer is only coupled to the top surface states, whereas its coupling with the bottom surface is ignored. Here, we will discuss how the torque is modified if the itinerant electron on the bottom surface may also couple to the FM, but with a weaker exchange coupling \({J}_{ex}^{^{\prime} }=\lambda {J}_{ex}\), i.e., with λ ≤ 1. In this case, the Hamiltonian of the bottom surface state becomes \({ {\mathcal H} }_{{\rm{TI}}}+\lambda {J}_{{\rm{ex}}}{\bf{m}}\cdot \hat{\sigma }\). The torque field is read as \({{\bf{H}}}^{{\rm{eff}}}={\eta }_{\lambda }(\hat{z}\times {{\bf{j}}}_{e}^{ss})\), where
It is easy to see that the coupling between the bottom surface and the ferromagnet leads to a reduction in the total spin torque, and it even vanishes for λ = 1. This results from the cancellation of the two surface states with opposite helicities. The equal exchange coupling is only possible if the film is extremely thin. In practice, this would not be the case since the film thickness should not be smaller than the effective thickness of the TSS (2 nm).
Weak exchange limit
In the previous section, we have evaluated the spin torque and the thickness optimization in the strong exchange limit. Similarly, we can estimate the optimal thickness in the weak exchange limit, \({J}_{{\rm{ex}}}\ll \hslash {v}_{{\rm{F}}}{k}_{{\rm{F}}}\). In this case, the torque field is derived as
Assuming the same distribution of the charge current in the system, the optimal thickness is calculated as \({d}_{{\rm{\max }}}=\sqrt{{\pi }^{2}{B}_{1}/\hslash {v}_{{\rm{F}}}{k}_{{\rm{F}}}}\). With the Fermi momentum k _{ F } = 0.07–0.14Å^{−1} ^{18, 26}, and the Fermi velocity v _{ F } ~ 5 × 10^{5} m/s^{21}, the optimal thickness is estimated to be in the range of ~1.4–2 nm. This range is almost below the effective thickness of the TI surface state, and thus the optimal spin torque may not be observed in the weak exchange regime.
Conclusion
In this paper, we have analytically derived the spinorbit torque induced by a thin TI film. First, we showed that in thin TI films, the spin torque is reduced due to the surface hybridization effect. This decrease is a consequence of the opposite helicities of the surface states on the two surfaces. On the other hand, lowering the thickness of the TI film may have a positive effect on the spin torque by reducing the bulk channel contribution to the total conductance. This increases the proportion of current flowing through the surface states, which constitutes the source of the currentinduced torque on the magnetic layer. Due to these opposing trends, there thus exists an optimal TI thickness at which the torque efficiency is maximized. Based on typical experimental parameter values, we found the torque efficiency at the optimal thickness to be several times larger than the torque values at the thick TIlayer limit. Our prediction for the optimal thickness is within the practical range which can be verified experimentally.
References
 1.
Tan, S. G., Jalil, M. B. A., Liu, X.J. & Fujita, T. Nonabelian gauge field effects and its relevance to spinning particle dynamics in the technology of spintronics. arXiv:0705.3502 (2007).
 2.
Tan, S. G., Jalil, M. B. A., Fujita, T. & Liu, X.J. Nonabelian gauge field effects and its relevance to spinning particle dynamics in the technology of spintronics. Ann. Phys. (NY) 326, 207, doi:10.1088/09538984/20/11/115206 (2011).
 3.
Manchon, A. & Zhang, S. Theory of nonequilibrium intrinsic spin torque in a single nanomagnet. Phys. Rev. B 78, 212405, doi:10.1103/PhysRevB.78.212405 (2008).
 4.
MatosAbiague, A. & RodrguezSuárez, R. L. Spinorbit coupling mediated spin torque in a single ferromagnetic layer. Phys. Rev. B 80, 094424, doi:10.1103/PhysRevB.80.094424 (2009).
 5.
Miron, I. M. et al. Currentdriven spin torque induced by the rashba effect in a ferromagnetic metal layer. Nat. Mater. 9, 230–234, doi:10.1038/nmat2613 (2010).
 6.
Li, H. et al. Intraband and interband spinorbit torques in noncentrosymmetric ferromagnets. Phys. Rev. B 91, 134402, doi:10.1103/PhysRevB.91.134402 (2015).
 7.
Haney, P. M., Lee, H.W., Lee, K.J., Manchon, A. & Stiles, M. D. Current induced torques and interfacial spinorbit coupling: Semiclassical modeling. Phys. Rev. B 87, 174411, doi:10.1103/PhysRevB.93.174421 (2013).
 8.
Kurebayashi, H. et al. An antidamping spinorbit torque originating from the berry curvature. Nat. Nanotechnol. 9, 211–217, doi:10.1038/nnano.2014.15 (2014).
 9.
Mihai Miron, I. et al. Currentdriven spin torque induced by the rashba effect in a ferromagnetic metal layer. Nat. Mater. 9, 230–234, doi:10.1038/nmat2613 (2010).
 10.
Mellnik, A. et al. Spintransfer torque generated by a topological insulator. Nature 511, 449–451, doi:10.1038/nature13534 (2014).
 11.
Wang, Y. et al. Topological surface states originated spinorbit torques in bi2se3. Phys. Rev. Lett 114, 257202, doi:10.1103/PhysRevLett.114.257202 (2015).
 12.
Fan, Y. et al. Magnetization switching through giant spin–orbit torque in a magnetically doped topological insulator heterostructure. Nat. Mater. 13, 699–704, doi:10.1038/nmat3973 (2014).
 13.
Edelstein, V. M. Spin polarization of conduction electrons induced by electric current in twodimensional asymmetric electron systems. Solid State Communications 73, 233–235, doi:10.1016/00381098(90)90963C (1990).
 14.
Murakami, S., Nagaosa, N. & Zhang, S.C. Dissipationless quantum spin current at room temperature. Science 301, 1348–1351, doi:10.1126/science.1087128 (2003).
 15.
Fujita, T., Jalil, M. & Tan, S. Unified description of intrinsic spinhall effect mechanisms. New J. Phys. 12, 013016, doi:10.1088/13672630/12/1/013016 (2010).
 16.
Kuroda, K. et al. Hexagonally deformed fermi surface of the 3d topological insulator bi2se3. Phys. Rev. Lett. 105, 076802, doi:10.1103/PhysRevLett.105.076802 (2010).
 17.
Linder, J., Yokoyama, T. & Sudbø, A. Anomalous finite size effects on surface states in the topological insulator bi2se3. Phys. Rev. B 80, 205401, doi:10.1103/PhysRevB.80.205401 (2009).
 18.
Bansal, N., Kim, Y. S., Brahlek, M., Edrey, E. & Oh, S. Thicknessindependent transport channels in topological insulator bi2se3 thin films. Phys. Rev. Lett 109, 116804, doi:10.1103/PhysRevLett.109.116804 (2012).
 19.
Zhang, G. et al. Quintuplelayer epitaxy of thin films of topological insulator bi2se3. Appl. Phys. Lett. 95, 053114, doi:10.1063/1.3200237 (2009).
 20.
Peng, H. et al. Aharonovbohm interference in topological insulator nanoribbons. Nat. Mater. 9, 225–229, doi:10.1038/nmat2609 (2010).
 21.
Zhang, Y. et al. Crossover of the threedimensional topological insulator bi2se3 to the twodimensional limit. Nat. Phys. 6, 584–588, doi:10.1038/nphys1779 (2010).
 22.
Lu, H.Z., Shan, W.Y., Yao, W., Niu, Q. & Shen, S.Q. Massive dirac fermions and spin physics in an ultrathin film of topological insulator. Phys. Rev. B 81, 115407, doi:10.1103/PhysRevB.81.115407 (2010).
 23.
Liu, C.X. et al. Oscillatory crossover from twodimensional to threedimensional topological insulators. Phys. Rev. B 81, 041307, doi:10.1103/PhysRevB.81.041307 (2010).
 24.
Zyuzin, A., Hook, M. & Burkov, A. Parallel magnetic field driven quantum phase transition in a thin topological insulator film. Phys. Rev. B 83, 245428, doi:10.1103/PhysRevB.83.245428 (2011).
 25.
Pershoguba, S. S. & Yakovenko, V. M. Spinpolarized tunneling current through a thin film of a topological insulator in a parallel magnetic field. Phys. Rev. B 86, 165404, doi:10.1103/PhysRevB.86.165404 (2012).
 26.
Hoefer, K. et al. Intrinsic conduction through topological surface states of insulating bi2te3 epitaxial thin films. PNAS 111, 14979–14984, doi:10.1073/pnas.1410591111 (2014).
Acknowledgements
We acknowledge the financial support of MOE Tier II grants MOE2013T22125 (NUS Grant No. R263000B10112) and R263000B98112, and the National Research Foundation of Singapore under the CRP Programs “Next Generation Spin Torque Memories: From Fundamental Physics to Applications” NRFCRP12201301 and “NonVolatile Magnetic Logic and Memory Integrated Circuit Devices” NRFCRP9201101.
Author information
Affiliations
Contributions
C.H. conceived the idea, carried out the analytical calculations, and wrote the manuscript. C.H., Y.W., Z.S., S.T., and M.J. analyzed the results. M.J. and H.Y. supervised the project. All authors reviewed the manuscript.
Corresponding author
Correspondence to Cong Son Ho.
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Received
Accepted
Published
DOI
Further reading

Spin accumulation in topological insulator thin films—influence of bulk and topological surface states
Journal of Physics D: Applied Physics (2018)

Highly Efficient SpintoCharge Current Conversion in Strained HgTe Surface States Protected by a HgCdTe Layer
Physical Review Letters (2018)

Impurity controlled crystal growth in low dimensional bismuth telluride
Chemistry of Materials (2018)

Spinorbit torque in a threedimensional topological insulator–ferromagnet heterostructure: Crossover between bulk and surface transport
Physical Review B (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.